- Fuel Cell Cars
- Fuel Cell Stacks
Fuel Cell Testing
- - Fixed Testing Systems
- - Liquid and Gas Delivery Systems
- - Fuel Cell Testing Hardware
- - Modular Testing Systems
- - Vacuum Tables and Temperature Controllers
- - Electronic Measurement and Control
- - Stack Humidification Systems
- - Ion Exchange Filters
- - Fuel Cell Testing Components
- - Portable Generators
- - Electrochemical Experiments
- Fuel Cell Components
- Hydrogen Equipment
- Power Devices
- Solar Power
- Hydro Power
- Wind Power
- Bioenergy Power
- Lab Accessories
- STEM Education
- Oxygen Devices
Toray Paper 090 - TGP-H-090 - is a carbon fiber composite paper suitable for use as a catalyst backing layer. It has a total thickness of 280 um (microns). Toray Paper 090 is a great low-cost alternative to conventional woven carbon cloth Gas Diffusion Layer (GDL) materials.
Toray carbon paper 090 comes with a standard 5% weight wet proofing. The Teflon gives the carbon material a hydrophobic property to better function as an electrode backing material.
This Toray Carbon Paper 090 value pack contains 9 - 10 x 10 cm sheets.
Lead time may be four to five business days.
*** By purchasing this good you agree that you will use the good(s) and their replicas for civilian use only, as described above, and you will never use them for the development or manufacture of weapons of mass destruction such as nuclear, biological or chemical weapons and missiles. If you decide to use the goods for any other application(s), you will immediately notify FuelCellsEtc in writing before using the goods in such other application(s).
|Gas Diffusion Layer Properties|
|Material Type||Carbon Fiber Paper|
|Thickness||.28 mm (280 microns)|
|Bulk Density||.44 g/cm3|
|Electrical Resistivity (through plane)||80 mΩcm|
|Flexural Strength (MPa)||40|
|Flexural Modulus (GPa)||10|
|Surface Roughness Ra||8 µm (microns)|
|Electrical Resistivity (in plane)||5.6 mΩcm|
|Thermal Conductivity (through plane, room temp)||(1.7) W/ (mk)|
|Thermal Conductivity (inplane, room temp)||21 W/ (mk)|
|Thermal Conductivity (inplane, 100°C)||23W/ (mk)|
|Coefficient of thermal expansion in plane||-0.8|
|PTFE Treatment||5 wt% (Standard)|
Write a review
Your Review: Note: HTML is not translated!
Rating: Bad Good
Enter the code in the box below: